3D model (JSmol)
|Molar mass||210.49 g/mol|
|Density||9.68 g/cm3, solid|
|Melting point||2,758 °C (4,996 °F; 3,031 K)|
|Boiling point||5,400 °C (9,750 °F; 5,670 K)|
Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).
|what is ?)(|
Hafnium(IV) oxide is the inorganic compound with the formula HfO2. Also known as hafnia, this colourless solid is one of the most common and stable compounds of hafnium. It is an electrical insulator with a band gap of 5.3~5.7 eV. Hafnium dioxide is an intermediate in some processes that give hafnium metal.
Hafnium(IV) oxide is quite inert. It reacts with strong acids such as concentrated sulfuric acid and with strong bases. It dissolves slowly in hydrofluoric acid to give fluorohafnate anions. At elevated temperatures, it reacts with chlorine in the presence of graphite or carbon tetrachloride to give hafnium tetrachloride.
Hafnia adopts the same structure as zirconia (ZrO2). Unlike TiO2, which features six-coordinate Ti in all phases, zirconia and hafnia consists of seven-coordinate metal centres. A variety of crystalline phases have been experimentally observed, including cubic (Fm-3m), tetragonal (P42/nmc), monoclinic (P21/c) and orthorhombic (Pbca and Pnma). It is also known that hafnia may adopt two other orthorhombic metastable phases (space group Pca21 and Pmn21) over a wide range of pressures and temperatures, presumably being the sources of the ferroelectricity recently observed in thin films of hafnia.
Thin films of hafnium oxides, used in modern semiconductor devices, are often deposited with an amorphous structure (commonly by atomic layer deposition). Possible benefits of the amorphous structure have led researchers to alloy hafnium oxide with silicon (forming hafnium silicates) or aluminium, which were found to increase the crystallization temperature of hafnium oxide.
Hafnia is used in optical coatings, and as a high-κ dielectric in DRAM capacitors and in advanced metal-oxide-semiconductor devices. Hafnium-based oxides were introduced by Intel in 2007 as a replacement for silicon oxide as a gate insulator in field-effect transistors. The advantage for transistors is its high dielectric constant: the dielectric constant of HfO2 is 4–6 times higher than that of SiO2. The dielectric constant and other properties depend on the deposition method, composition and microstructure of the material.
In recent years, hafnium oxide (as well as doped and oxygen-deficient hafnium oxide) attracts additional interest as a possible candidate for resistive-switching memories and CMOS-compatible ferroelectric field effect transistors and memory chips.
Multilayered films of hafnium dioxide, silica, and other materials have been developed for use in passive cooling of buildings. The films reflect sunlight and radiate heat at wavelengths that pass through Earth's atmosphere, and can have temperatures several degrees cooler than surrounding materials under the same conditions.
- Bersch, Eric; et al. (2008). "Band offsets of ultrathin high-k oxide films with Si". Phys. Rev. B. 78 (8): 085114. Bibcode:2008PhRvB..78h5114B. doi:10.1103/PhysRevB.78.085114.
- Table III, V. Miikkulainen; et al. (2013). "Crystallinity of inorganic films grown by atomic layer deposition: Overview and general trends". Journal of Applied Physics. 113 (2): 021301–021301–101. Bibcode:2013JAP...113b1301M. doi:10.1063/1.4757907.
- T. D. Huan; V. Sharma; G. A. Rossetti, Jr.; R. Ramprasad (2014). "Pathways towards ferroelectricity in hafnia". Physical Review B. 90 (6): 064111. arXiv:1407.1008. Bibcode:2014PhRvB..90f4111H. doi:10.1103/PhysRevB.90.064111.
- T. S. Boscke (2011). "Ferroelectricity in hafnium oxide thin films". Applied Physics Letters. 99 (10): 102903. Bibcode:2011ApPhL..99j2903B. doi:10.1063/1.3634052.
- J.H. Choi; et al. (2011). "Development of hafnium based high-k materials—A review". Materials Science and Engineering: R. 72 (6): 97–136. doi:10.1016/j.mser.2010.12.001.
- H. Zhu; C. Tang; L. R. C. Fonseca; R. Ramprasad (2012). "Recent progress in ab initio simulations of hafnia-based gate stacks". Journal of Materials Science. 47 (21): 7399–7416. Bibcode:2012JMatS..47.7399Z. doi:10.1007/s10853-012-6568-y.
- Intel (11 November 2007). "Intel's Fundamental Advance in Transistor Design Extends Moore's Law, Computing Performance".
- Wilk G. D., Wallace R. M., Anthony J. M. (2001). "High-κ gate dielectrics: Current status and materials properties considerations". Journal of Applied Physics. 89 (10): 5243–5275. Bibcode:2001JAP....89.5243W. doi:10.1063/1.1361065. , Table 1
- K.-L. Lin; et al. (2011). "Electrode dependence of filament formation in HfO2 resistive-switching memory". Journal of Applied Physics. 109 (8): 084104–084104–7. Bibcode:2011JAP...109h4104L. doi:10.1063/1.3567915.
- Imec (7 June 2017). "Imec demonstrates breakthrough in CMOS-compatible Ferroelectric Memory".
- The Ferroelectric Memory Company (8 June 2017). "World's first FeFET-based 3D NAND demonstration".
- T. S. Böscke, J. Müller, D. Bräuhaus (7 Dec 2011). "Ferroelectricity in hafnium oxide: CMOS compatible ferroelectric field effect transistors". 2011 International Electron Devices Meeting. IEEE. doi:10.1109/IEDM.2011.6131606.
- Nivole Ahner (August 2018). Mit HFO2 voll CMOS-kompatibel (in German). Elektronik Industrie.
- Very High Temperature Exotic Thermocouple Probes product data, Omega Engineering, Inc., retrieved 2008-12-03
- "Aaswath Raman | Innovators Under 35 | MIT Technology Review". August 2015. Retrieved 2015-09-02.